- Home
- Documents
*Intrinsic viscosities and osmotic molecular weights of ... The osmotic-pressure values for all the*

prev

next

out of 7

View

215Download

0

Embed Size (px)

U. S. D EPARTMENT OP COMMERCE NATIONAL BUREAU OF STANDARDS

RESEARCH PAPER RP1654

Part of Journal of Research of the N.ational Bureau of Standards, Volume 34, May 1945

INTRINSIC VISCOSITIES AND OSMOTIC MOLECULAR WEIGHTS OF CELLULOSE ACETATE FRACTIONS

By Arnold M. Sookne and Milton Harris 1

ABSTRACT

The intrinsic viscosities and osmotically estimated number-average molecular weights of a series of cellulose acetate fractions have been measured. It was found that within t he range of chain lengths investigated (number-average molecular weight, lvin, up to 130,000) the number-average molecular weights are proportional to the intrinsic viscosities in acetone solu t ions, in agreement with Staudinger's rule and the results of Kraemer. An estimate is provided of the r elative homogeneity with respect to molecular size of the fraction s and the starting material from which they were prepared.

CONTENTS Page

I. Introduction ______ __________ _______ __ ___ __ __ ______ __ ______ _____ _ 459 II. 11ethods __ __ __________________ _____ ___________ _________ ______ __ 460

1. Viscosity measurements _____ _____________________________ _ 460 2. Osmotic-pressure measurements _ _ _ _ _ _ _ _ _ _ _ _ _ _ _ _ _ _ _ _ _ _ _ _ _ _ _ _ 460

III. R esults and discussion _______ _____ __ ___________ ________ ___ _______ 461 IV. R eferences ________ ___________ ____ ___ _________________ ___ __ __ ____ 465

I. INTRODUCTION

According to Staudinger's rule, the molecular weight, M, of a linear high polymer is related to its intrinsic viscosity, b]' by the expression

[7]]=KM, where [7]]=~~~ (7]rp/C), K is a constant, and C the concentra-tion in grams per 100 ml of solution [1).2 The validity of this relation-ship has often been questioned, and it has recently been demonstrated that several unbranched polymers do not conform to this rule but rather to the more general relationship [7]]=KMa, where a is a constant with a value between 0.5 and 2 [2, 3].

Some time ago a series of cellulose acetate fractions was prepared in this laboratory in connection with a study of the mechanical prop-erties of this material [4].3 The intrinsic viscosities and the osmot-ically estimated molecular weights of these fractions and of the start-ing material have now been determined in acetone solutions. This

1 Research Associates at the National Bureau ol Standards, representing tbe Textile Foundation. , Figures in brackets indicate literature relerences at tbe end ol tbis paper . The starting materiallrom wbicb the fractions were prepared had an acetyl content ol 38.6 percent, an

asb ol 0.06 percent, a melting pOint ol 250 C and a cbar point ol 301 C.

459

460 J owrnal of Researoh of the National Bureau of Standards

paper, which presents the results of these measurements, shows that for this type of acetate and within the range of chain lengths inves-tigated, the system cellulose acetate in acetone does conform to Staudinger's rule; i. e., for this system the constant a has the value unity in the relationship cited above.

II. METHODS

1. VISCOSITY MEASUREMENTS

The viscosity measurements were made in an Ostwald viscometer at 25O.03 C . . As the time of efflux of the acetone was approxi-matelyonly 30 seconds, kinetic-energy corrections were applied 4 [5]. These were determined by calibrating the viscometer with oils of known viscosity obtained at the National Bureau of Standards.

2. OSMOTIC-PRESSURE MEASUREMENTS

The osmotic-pressure values for all the fractions, except the one of lowest molecular weight, were determined by the dynamic method of Fuoss and Mead [6]. The denitrnted cellulose nitrate membranes recommended by these authors were used. The measurements were made at room temperature (approximately 28 C.). The cell was placed in a box insulated with cotton waste, and the entire assembly was then covered with a wooden hood to minimize drifts caused by changes in temperature. Measurements of the osmotic pressures were made by means of a cathetometer sighted through a window in the hood. It was found practical to use the same membrane for a series of measurements by using increasing concentrations of the same sample in successive measurements, as recommended by Fuoss and Mead [6]. The membrane was then rinsed thoroughly with acetone, soaked overnight in this solvent, and rinsed thoroughly again, all without removing the membrane from the cell. This treatment suf-ficed to remove adhering cellulose acetate, so that the membrane could be used again.

With the fraction of lowest molecular weight (15), and to a lesser extent with the starting material, appreciable diffusion of the solute through the denitrated cellulose nitrate membranes occurred. For these two samples, cellophane membranes, swollen with NH40H according to the directions of Flory [2], were therefore used. These measurements were made by the static method in a constant-tem-perature room. Equilibrium was reached overnight, after which no appreciable change in osmotic pressure occurred for a period of several days.

As the osmotic pressure measurements were made at slightly dif-ferent temperatures, the values of Mn were calculated as follows: The apparent value of Mn at each concentration (and corresponding temperature) was first calculated by using the van't Hoff relationship, and the value of Un at zero concentration was then obtained alge-braically, assuming that the apparent value of Mn is a linear function of concentration.

I Failure to apply kinetic energy corrections leads to errors of several percent in the values of the intrinsic viscosities of the fractions of higher molecular weight.

Molecular Weight of OellJulose Acetate 461

III. RESULTS AND DISCUSSION

The results of the viscosity measurements are presented in table 1 and shown graphically in figure 1. In this figure the values of 'YIsp /c are plotted on a logarithmic scale. When this procedure is followed, the results fall on straight lines suitable for extrapolation to zero concentration for obtaining the intrinsic viscosity. (When

-l :::;:

>-0 !:::o ~, ol? ~z >0

7.---------,---------,---------,---------~

:3 5~-----~---1----------~~2~~~--_r----------~

10

~_---iI12

i= 2(2 !:!:~

u z t==::::::~~==~===13===f==~.~----_r----------l if ~ .7 914 VlZ o '-'

.5r---------+---------+---------1---------~

~-------+-..------_+-o15

FRACTIONS o STARTING

MATERIAL

.20~------~.2~5~--------~.5hO~--------~7~5--------~I.OO

CONCENTRATION, G/IOO ML

FIGURE 1.- Viscosity-concentration relationship in acetone solutions for cellulose acetate samples.

Tbe samples are numbered in the order of tbeir molecular weigbts to conform witb tbeir designations in a. previous publication [4] . Tbe lowest number represents tbe sample of highest molecular weight.

the values of 'YIsp /c and c are both plotted on a linear scale, the results do not fall on straight lines except at very low concentrations, where the experimental errors are largest. The use of the semilogarithmic plot gives weight to the more precisely determined values obtained in the range of higher concentrations).

The result of the viscosity measurements conform quite closely to Martin's equation [7]:

log 'YIC'=log(1)] + kb] a, (1)

in which a is the concentration/ and k is a constant characteristic of a given polymeric series in a given solvent. The values of (1)] given

, It should be noted tbat tbe concentration is expressed in g/lOO ml of solution in the data presented bere. wbereas it is given in weigbt'percent in reference [71.

462 Journal of Research of the National Bureau of Standards

in table 1 were obtained by algebraic extrapolation, using the method of least squares.

TABLE 1.-Viscosities of cellulose acetate samples in acetone solutions at 25 C

(The samples are numbered in the order of their molecular weights to conform with tbeir designations in a previous publication [4]. The lowest number represents the sample oC bigbest molecular weigbt.]

Sample Concentra-tion

U/l00 ml

~ ..

Starting materiaL ____ . ----- --- --- -------- ----- -- --- -- - r---o~ ~~- ---- --~~Mr --. ----11 Fraction:

2.. ____ ___ -- ------------------------------------ - {" -- --~~r ---- -- ~~~~- ------T~r 3.. -- - -------- -- - --- -- -- -. -- ---- --- -- ----- ---- -- - -- -r---]~- -- ----r~~ ----- ---nr 4_ --- ---- ---- -- ----- ------ -- ---- -- ---- ---- -- -- -- -- -- f---- -~~gr -- ---T~~- -- ----l!r 5_ -- -- --- -- ---- -- --- ------ -- -. -- -- ---- ---- -- ----- --- f -----~ ~~- ------n~~- ---- -- -~l 6 ____ __ ______ -- ------ -- ---- -- -- -- ---- ---- --- ---- ---- r----~~~- ------~~ ~r -- -----nr 7.. ___ ----- --------- -- -- -- -- -- -- -- -- ---- ------ ---- -- {' -- --]~- ---- --~]~- -------rH-8_ - - - ---- ------ -- ---- ----- -- -. -- -- -- -- -- -- --- ---- ---1------:-gf ---- --0: ~~- -- -- ---nr

. 428 _ 88, 2. 07

9.. __ _ -- - - ---- - ------- - ------ ------- -- ------ -------- { -- - --]!r --- -- --]~- -- -----~1 10 ________ -- ---- -- ------ ---- - -------------- -- -- --- -- {"-- -- ~ Hr -- -- -- ~~ ~r -------~l 11 _ ----- -- --- -- -. --- - - - -- - ---------- -- -- -- -- - -- - ---- {- -- - - -~ ~J -- -- -- o~ ur -- -- --T~-12.. __________ -------- -- -- -- ------- ----------------- {" ----~ Hr ---- --- ~ nr -- -----~l 13_ -- - -- -- --- -- - -- -- --- --- --- --- -- --- --,-- -- - --- --- - {--- -- - ~ ~- ---- --- ~ !~r -- ---- -o~~r 14 . . - --- . --- --- --. -- --- -- -- - . --- ----- -- --- - - -- --- . -- {------~llr ------ -~ ~~- -- -- -- --~~-15.. -- -- -- ------------ - -------- -- -- ------- -- ------ -- { ---- --: ~r~ --- -----: ~r -